#------------------------------------------------------------------------------
#$Date: 2021-04-14 12:47:21 +0300 (Wed, 14 Apr 2021) $
#$Revision: 264145 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/17/1561750.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561750
loop_
_publ_author_name
'Bykova, E.'
'Gou, H.'
'Bykov, M.'
'Hanfland, M.'
'Dubrovinsky, L.'
'Dubrovinskaia, N.'
_publ_section_title
;
 Crystal structures and compressibility of novel iron borides Fe2B7 and Fe
 B50 synthesized at high pressure and high temperature
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              102
_journal_page_last               109
_journal_paper_doi               10.1016/j.jssc.2015.06.040
_journal_volume                  230
_journal_year                    2015
_chemical_absolute_configuration .
_chemical_formula_moiety         'B50 Fe1.324'
_chemical_formula_sum            'B50 Fe1.324'
_chemical_formula_weight         614.4
_chemical_name_common            'Iron Boron (1.324/50)'
_chemical_name_systematic        'Iron Boron (1.324/50)'
_space_group_IT_number           134
_space_group_name_Hall           '-P 4ac 2bc'
_space_group_name_H-M_alt        'P 42/n n m :2'
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      134
_symmetry_space_group_name_Hall  '-P 4ac 2bc'
_symmetry_space_group_name_H-M   'P 42/n n m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   8.6807(3)
_cell_length_b                   8.6807(3)
_cell_length_c                   4.9043(2)
_cell_measurement_reflns_used    290
_cell_measurement_temperature    293
_cell_measurement_theta_max      18.26
_cell_measurement_theta_min      3.1
_cell_volume                     369.56(2)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_structure_refinement  'Jana2006 (Petricek, 2014)'
_computing_structure_solution    'SHELXS-2013 (Sheldrick, 2013)'
_diffrn_ambient_pressure         22100000
_diffrn_ambient_temperature      293
_diffrn_detector                 'MAR555 flatpanel detector'
_diffrn_measured_fraction_theta_full 0.92
_diffrn_measured_fraction_theta_max 0.66
_diffrn_measurement_device
;
customized omega-circle diffractometer
;
_diffrn_measurement_device_type  'ESRF, beamline ID09A diffractometer'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.41409
_diffrn_reflns_av_R_equivalents  0.054
_diffrn_reflns_av_unetI/netI     0.0355
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            831
_diffrn_reflns_theta_full        13.88
_diffrn_reflns_theta_max         19.46
_diffrn_reflns_theta_min         2.73
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    0.31
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.615
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.76
_exptl_crystal_description       plate
_exptl_crystal_F_000             284
_exptl_crystal_size_max          0.020
_exptl_crystal_size_mid          0.010
_exptl_crystal_size_min          0.005
_refine_diff_density_max         0.65
_refine_diff_density_min         -0.60
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    2.82
_refine_ls_goodness_of_fit_ref   2.65
_refine_ls_number_constraints    0
_refine_ls_number_parameters     35
_refine_ls_number_reflns         289
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0633
_refine_ls_R_factor_gt           0.0595
_refine_ls_shift/su_max          0.0002
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(σ²(I)+0.0004I²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1282
_refine_ls_wR_factor_ref         0.1295
_reflns_number_gt                255
_reflns_number_total             289
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            fe1.32B50_22.1GPa.cif
_cod_data_source_block           Fe1.3B50_22.1GPa
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the built-in table derived from the CIF
Core dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      'P 42/n n m'
_cod_database_code               1561750
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -x+1/2,-y+1/2,z
3 -y+1/2,x,z+1/2
4 y,-x+1/2,z+1/2
5 -x+1/2,y,-z+1/2
6 x,-y+1/2,-z+1/2
7 y,x,-z
8 -y+1/2,-x+1/2,-z
9 -x,-y,-z
10 x+1/2,y+1/2,-z
11 y+1/2,-x,-z+1/2
12 -y,x+1/2,-z+1/2
13 x+1/2,-y,z+1/2
14 -x,y+1/2,z+1/2
15 -y,-x,z
16 y+1/2,x+1/2,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe -0.25 0.25 0.25 Uani 0.0140(4) 2 0.6621 d . . .
B4 B -0.0760(3) -0.1585(4) 0.1499(5) Uani 0.0121(8) 16 1 d . . .
B5 B -0.1681(3) 0.0211(3) 0.1621(5) Uani 0.0110(8) 16 1 d . . .
B2 B 0.1234(3) -0.1234(3) 0.1406(7) Uani 0.0107(8) 8 1 d . . .
B3 B 0.0035(3) -0.0035(3) 0.3359(7) Uani 0.0097(8) 8 1 d . . .
B1 B 0.25 -0.25 0.25 Uani 0.0102(16) 2 1 d . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B -0.0003 0.0002 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Fe 0.1988 0.3099 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
B5 Fe1 B5 . . 2_455 156.91(9)
B5 Fe1 B5 . . 5_455 45.40(11)
B5 Fe1 B5 . . 6_555 141.47(11)
B5 Fe1 B5 . . 11_455 92.30(11)
B5 Fe1 B5 . . 12_555 92.30(11)
B5 Fe1 B5 . . 15_555 49.54(11)
B5 Fe1 B5 . . 16_455 124.66(11)
B5 Fe1 B2 . . 3_455 83.77(10)
B5 Fe1 B2 . . 4_555 114.80(10)
B5 Fe1 B2 . . 7_555 44.49(10)
B5 Fe1 B2 . . 8_455 113.74(10)
B5 Fe1 B1 . . 3_454 78.46(7)
B5 Fe1 B1 . . 3_455 101.54(7)
B5 Fe1 B5 2_455 . 5_455 141.47(11)
B5 Fe1 B5 2_455 . 6_555 45.40(11)
B5 Fe1 B5 2_455 . 11_455 92.30(11)
B5 Fe1 B5 2_455 . 12_555 92.30(11)
B5 Fe1 B5 2_455 . 15_555 124.66(11)
B5 Fe1 B5 2_455 . 16_455 49.54(11)
B5 Fe1 B2 2_455 . 3_455 114.80(10)
B5 Fe1 B2 2_455 . 4_555 83.77(10)
B5 Fe1 B2 2_455 . 7_555 113.74(10)
B5 Fe1 B2 2_455 . 8_455 44.49(10)
B5 Fe1 B1 2_455 . 3_454 78.46(7)
B5 Fe1 B1 2_455 . 3_455 101.54(7)
B5 Fe1 B5 5_455 . 6_555 156.91(9)
B5 Fe1 B5 5_455 . 11_455 49.54(11)
B5 Fe1 B5 5_455 . 12_555 124.66(11)
B5 Fe1 B5 5_455 . 15_555 92.30(11)
B5 Fe1 B5 5_455 . 16_455 92.30(11)
B5 Fe1 B2 5_455 . 3_455 44.49(10)
B5 Fe1 B2 5_455 . 4_555 113.74(10)
B5 Fe1 B2 5_455 . 7_555 83.77(10)
B5 Fe1 B2 5_455 . 8_455 114.80(10)
B5 Fe1 B1 5_455 . 3_454 101.54(7)
B5 Fe1 B1 5_455 . 3_455 78.46(7)
B5 Fe1 B5 6_555 . 11_455 124.66(11)
B5 Fe1 B5 6_555 . 12_555 49.54(11)
B5 Fe1 B5 6_555 . 15_555 92.30(11)
B5 Fe1 B5 6_555 . 16_455 92.30(11)
B5 Fe1 B2 6_555 . 3_455 113.74(10)
B5 Fe1 B2 6_555 . 4_555 44.49(10)
B5 Fe1 B2 6_555 . 7_555 114.80(10)
B5 Fe1 B2 6_555 . 8_455 83.77(10)
B5 Fe1 B1 6_555 . 3_454 101.54(7)
B5 Fe1 B1 6_555 . 3_455 78.46(7)
B5 Fe1 B5 11_455 . 12_555 156.91(9)
B5 Fe1 B5 11_455 . 15_555 141.47(11)
B5 Fe1 B5 11_455 . 16_455 45.40(11)
B5 Fe1 B2 11_455 . 3_455 44.49(10)
B5 Fe1 B2 11_455 . 4_555 113.74(10)
B5 Fe1 B2 11_455 . 7_555 114.80(10)
B5 Fe1 B2 11_455 . 8_455 83.77(10)
B5 Fe1 B1 11_455 . 3_454 101.54(7)
B5 Fe1 B1 11_455 . 3_455 78.46(7)
B5 Fe1 B5 12_555 . 15_555 45.40(11)
B5 Fe1 B5 12_555 . 16_455 141.47(11)
B5 Fe1 B2 12_555 . 3_455 113.74(10)
B5 Fe1 B2 12_555 . 4_555 44.49(10)
B5 Fe1 B2 12_555 . 7_555 83.77(10)
B5 Fe1 B2 12_555 . 8_455 114.80(10)
B5 Fe1 B1 12_555 . 3_454 101.54(7)
B5 Fe1 B1 12_555 . 3_455 78.46(7)
B5 Fe1 B5 15_555 . 16_455 156.91(9)
B5 Fe1 B2 15_555 . 3_455 114.80(10)
B5 Fe1 B2 15_555 . 4_555 83.77(10)
B5 Fe1 B2 15_555 . 7_555 44.49(10)
B5 Fe1 B2 15_555 . 8_455 113.74(10)
B5 Fe1 B1 15_555 . 3_454 78.46(7)
B5 Fe1 B1 15_555 . 3_455 101.54(7)
B5 Fe1 B2 16_455 . 3_455 83.77(10)
B5 Fe1 B2 16_455 . 4_555 114.80(10)
B5 Fe1 B2 16_455 . 7_555 113.74(10)
B5 Fe1 B2 16_455 . 8_455 44.49(10)
B5 Fe1 B1 16_455 . 3_454 78.46(7)
B5 Fe1 B1 16_455 . 3_455 101.54(7)
B2 Fe1 B2 3_455 . 4_555 78.10(10)
B2 Fe1 B2 3_455 . 7_555 127.09(10)
B2 Fe1 B2 3_455 . 8_455 127.09(10)
B2 Fe1 B1 3_455 . 3_454 140.95(7)
B2 Fe1 B1 3_455 . 3_455 39.05(7)
B2 Fe1 B2 4_555 . 7_555 127.09(10)
B2 Fe1 B2 4_555 . 8_455 127.09(10)
B2 Fe1 B1 4_555 . 3_454 140.95(7)
B2 Fe1 B1 4_555 . 3_455 39.05(7)
B2 Fe1 B2 7_555 . 8_455 78.10(10)
B2 Fe1 B1 7_555 . 3_454 39.05(7)
B2 Fe1 B1 7_555 . 3_455 140.95(7)
B2 Fe1 B1 8_455 . 3_454 39.05(7)
B2 Fe1 B1 8_455 . 3_455 140.95(7)
B1 Fe1 B1 3_454 . 3_455 180.0(5)
B4 B4 B4 6_545 . 7_555 140.7(2)
B4 B4 B5 6_545 . . 137.6(2)
B4 B4 B5 6_545 . 7_555 114.8(2)
B4 B4 B2 6_545 . . 99.3(2)
B4 B4 B3 6_545 . . 112.1(2)
B4 B4 B5 7_555 . . 59.26(15)
B4 B4 B5 7_555 . 7_555 59.45(16)
B4 B4 B2 7_555 . . 107.7(2)
B4 B4 B3 7_555 . . 106.1(2)
B5 B4 B5 . . 7_555 107.0(2)
B5 B4 B2 . . . 107.2(2)
B5 B4 B3 . . . 58.90(16)
B5 B4 B2 7_555 . . 60.73(17)
B5 B4 B3 7_555 . . 107.4(2)
B2 B4 B3 . . . 59.76(17)
Fe1 B5 B4 . . . 167.88(18)
Fe1 B5 B4 . . 7_555 129.46(17)
Fe1 B5 B5 . . 5_455 67.30(14)
Fe1 B5 B5 . . 15_555 65.23(13)
Fe1 B5 B2 . . 7_555 77.15(14)
Fe1 B5 B3 . . . 107.43(17)
B4 B5 B4 . . 7_555 61.29(16)
B4 B5 B5 . . 5_455 114.1(2)
B4 B5 B5 . . 15_555 107.8(2)
B4 B5 B2 . . 7_555 108.49(19)
B4 B5 B3 . . . 60.93(17)
B4 B5 B5 7_555 . 5_455 119.6(2)
B4 B5 B5 7_555 . 15_555 107.88(19)
B4 B5 B2 7_555 . 7_555 59.89(16)
B4 B5 B3 7_555 . . 109.3(2)
B5 B5 B5 5_455 . 15_555 127.2(2)
B5 B5 B2 5_455 . 7_555 128.4(2)
B5 B5 B3 5_455 . . 118.8(2)
B5 B5 B2 15_555 . 7_555 59.40(15)
B5 B5 B3 15_555 . . 58.55(16)
B2 B5 B3 7_555 . . 106.6(2)
Fe1 B2 B4 3_554 . . 112.43(18)
Fe1 B2 B4 3_554 . 15_555 112.43(18)
Fe1 B2 B5 3_554 . 7_555 58.36(13)
Fe1 B2 B5 3_554 . 9_555 58.36(13)
Fe1 B2 B3 3_554 . . 162.1(2)
Fe1 B2 B1 3_554 . . 69.99(11)
B4 B2 B4 . . 15_555 109.9(2)
B4 B2 B5 . . 7_555 59.37(16)
B4 B2 B5 . . 9_555 108.9(2)
B4 B2 B3 . . . 60.33(17)
B4 B2 B1 . . . 122.3(2)
B4 B2 B5 15_555 . 7_555 108.9(2)
B4 B2 B5 15_555 . 9_555 59.37(16)
B4 B2 B3 15_555 . . 60.33(17)
B4 B2 B1 15_555 . . 122.3(2)
B5 B2 B5 7_555 . 9_555 61.20(17)
B5 B2 B3 7_555 . . 106.8(2)
B5 B2 B1 7_555 . . 117.5(2)
B5 B2 B3 9_555 . . 106.8(2)
B5 B2 B1 9_555 . . 117.5(2)
B3 B2 B1 . . . 127.9(2)
B4 B3 B4 . . 15_555 109.2(2)
B4 B3 B5 . . . 60.17(17)
B4 B3 B5 . . 15_555 110.7(2)
B4 B3 B2 . . . 59.92(17)
B4 B3 B3 . . 7_556 122.0(2)
B4 B3 B5 15_555 . . 110.7(2)
B4 B3 B5 15_555 . 15_555 60.17(17)
B4 B3 B2 15_555 . . 59.92(17)
B4 B3 B3 15_555 . 7_556 122.0(2)
B5 B3 B5 . . 15_555 62.90(17)
B5 B3 B2 . . . 108.4(2)
B5 B3 B3 . . 7_556 117.0(2)
B5 B3 B2 15_555 . . 108.4(2)
B5 B3 B3 15_555 . 7_556 117.0(2)
B2 B3 B3 . . 7_556 126.1(2)
Fe1 B1 Fe1 3_554 . 3_555 180.0(5)
Fe1 B1 B2 3_554 . . 70.96(12)
Fe1 B1 B2 3_554 . 2_545 70.96(12)
Fe1 B1 B2 3_554 . 5_555 109.04(12)
Fe1 B1 B2 3_554 . 6_545 109.04(12)
Fe1 B1 B2 3_555 . . 109.04(12)
Fe1 B1 B2 3_555 . 2_545 109.04(12)
Fe1 B1 B2 3_555 . 5_555 70.96(12)
Fe1 B1 B2 3_555 . 6_545 70.96(12)
B2 B1 B2 . . 2_545 141.92(17)
B2 B1 B2 . . 5_555 96.11(15)
B2 B1 B2 . . 6_545 96.11(15)
B2 B1 B2 2_545 . 5_555 96.11(15)
B2 B1 B2 2_545 . 6_545 96.11(15)
B2 B1 B2 5_555 . 6_545 141.92(17)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
Fe1 B5 . . 2.154(3)
Fe1 B5 . 2_455 2.154(3)
Fe1 B5 . 5_455 2.154(3)
Fe1 B5 . 6_555 2.154(3)
Fe1 B5 . 11_455 2.154(3)
Fe1 B5 . 12_555 2.154(3)
Fe1 B5 . 15_555 2.154(3)
Fe1 B5 . 16_455 2.154(3)
Fe1 B2 . 3_455 2.467(3)
Fe1 B2 . 4_555 2.467(3)
Fe1 B2 . 7_555 2.467(3)
Fe1 B2 . 8_455 2.467(3)
Fe1 B1 . 3_454 2.4522(2)
Fe1 B1 . 3_455 2.4522(2)
B4 B4 . 6_545 1.868(4)
B4 B4 . 7_555 1.785(4)
B4 B5 . . 1.753(4)
B4 B5 . 7_555 1.749(4)
B4 B2 . . 1.758(4)
B4 B3 . . 1.766(4)
B5 B5 . 5_455 1.663(4)
B5 B5 . 15_555 1.805(4)
B5 B2 . 7_555 1.773(4)
B5 B3 . . 1.730(4)
B2 B3 . . 1.756(4)
B2 B1 . . 1.644(3)
B3 B3 . 7_556 1.612(5)
